LMucko/crystallography-open-database huggingface dataset:
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p1 Note: P = .22 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017119
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p1
 Note: P = .22 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7788
_cell_length_b                   4.7788
_cell_length_c                   15.685
_cell_formula_units_Z            6
_cell_volume                     310.208
_database_code_amcsd             0020358
_diffrn_ambient_pressure         2.2e+05
_exptl_crystal_density_diffrn    3.673
_cod_data_source_file            inputs/fixed/downloads/05/05840.cif
_cod_data_source_block           05840
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017119
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p2 Note: P = .79 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017120
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p2
 Note: P = .79 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7753
_cell_length_b                   4.7753
_cell_length_c                   15.6360
_cell_formula_units_Z            6
_cell_volume                     308.786
_database_code_amcsd             0020359
_diffrn_ambient_pressure         7.9e+05
_exptl_crystal_density_diffrn    3.690
_cod_data_source_file            inputs/fixed/downloads/05/05841.cif
_cod_data_source_block           05841
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017120
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p3 Note: P = 1.62 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017121
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p3
 Note: P = 1.62 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7714
_cell_length_b                   4.7714
_cell_length_c                   15.578
_cell_formula_units_Z            6
_cell_volume                     307.138
_database_code_amcsd             0020360
_diffrn_ambient_pressure         1.62e+06
_exptl_crystal_density_diffrn    3.709
_cod_data_source_file            inputs/fixed/downloads/05/05842.cif
_cod_data_source_block           05842
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017121
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p4 Note: P = 2.12 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017122
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p4
 Note: P = 2.12 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7654
_cell_length_b                   4.7654
_cell_length_c                   15.531
_cell_formula_units_Z            6
_cell_volume                     305.442
_database_code_amcsd             0020361
_diffrn_ambient_pressure         2.12e+06
_exptl_crystal_density_diffrn    3.730
_cod_data_source_file            inputs/fixed/downloads/05/05843.cif
_cod_data_source_block           05843
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017122
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p5 Note: P = 2.66 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017123
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p5
 Note: P = 2.66 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7581
_cell_length_b                   4.7581
_cell_length_c                   15.473
_cell_formula_units_Z            6
_cell_volume                     303.370
_database_code_amcsd             0020362
_diffrn_ambient_pressure         2.66e+06
_exptl_crystal_density_diffrn    3.756
_cod_data_source_file            inputs/fixed/downloads/05/05844.cif
_cod_data_source_block           05844
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017123
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p6 Note: P = 3.57 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017124
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p6
 Note: P = 3.57 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7426
_cell_length_b                   4.7426
_cell_length_c                   15.368
_cell_formula_units_Z            6
_cell_volume                     299.351
_database_code_amcsd             0020363
_diffrn_ambient_pressure         3.57e+06
_exptl_crystal_density_diffrn    3.806
_cod_data_source_file            inputs/fixed/downloads/05/05845.cif
_cod_data_source_block           05845
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017124
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p7 Note: P = 4.39 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017125
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p7
 Note: P = 4.39 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7409
_cell_length_b                   4.7409
_cell_length_c                   15.319
_cell_formula_units_Z            6
_cell_volume                     298.183
_database_code_amcsd             0020364
_diffrn_ambient_pressure         4.39e+06
_exptl_crystal_density_diffrn    3.821
_cod_data_source_file            inputs/fixed/downloads/05/05846.cif
_cod_data_source_block           05846
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017125
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p8 Note: P = 4.74 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017126
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p8
 Note: P = 4.74 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7415
_cell_length_b                   4.7415
_cell_length_c                   15.308
_cell_formula_units_Z            6
_cell_volume                     298.044
_database_code_amcsd             0020365
_diffrn_ambient_pressure         4.74e+06
_exptl_crystal_density_diffrn    3.823
_cod_data_source_file            inputs/fixed/downloads/05/05847.cif
_cod_data_source_block           05847
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017126
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p9 Note: P = 5.20 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017127
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p9
 Note: P = 5.20 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7388
_cell_length_b                   4.7388
_cell_length_c                   15.287
_cell_formula_units_Z            6
_cell_volume                     297.296
_database_code_amcsd             0020366
_diffrn_ambient_pressure         5.2e+06
_exptl_crystal_density_diffrn    3.832
_cod_data_source_file            inputs/fixed/downloads/05/05848.cif
_cod_data_source_block           05848
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017127
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p10 Note: P = 6.33 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017128
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p10
 Note: P = 6.33 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7332
_cell_length_b                   4.7332
_cell_length_c                   15.1926
_cell_formula_units_Z            6
_cell_volume                     294.763
_database_code_amcsd             0020367
_diffrn_ambient_pressure         6.33e+06
_exptl_crystal_density_diffrn    3.865
_cod_data_source_file            inputs/fixed/downloads/05/05849.cif
_cod_data_source_block           05849
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017128
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p11 Note: P = 7.01 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017129
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p11
 Note: P = 7.01 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7248
_cell_length_b                   4.7248
_cell_length_c                   15.1242
_cell_formula_units_Z            6
_cell_volume                     292.395
_database_code_amcsd             0020368
_diffrn_ambient_pressure         7.01e+06
_exptl_crystal_density_diffrn    3.897
_cod_data_source_file            inputs/fixed/downloads/05/05850.cif
_cod_data_source_block           05850
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017129
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p12 Note: P = 8.33 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017130
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p12
 Note: P = 8.33 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7177
_cell_length_b                   4.7177
_cell_length_c                   15.043
_cell_formula_units_Z            6
_cell_volume                     289.952
_database_code_amcsd             0020369
_diffrn_ambient_pressure         8.33e+06
_exptl_crystal_density_diffrn    3.929
_cod_data_source_file            inputs/fixed/downloads/05/05851.cif
_cod_data_source_block           05851
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017130
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p13 Note: P = 9.17 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017131
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p13
 Note: P = 9.17 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7146
_cell_length_b                   4.7146
_cell_length_c                   14.9903
_cell_formula_units_Z            6
_cell_volume                     288.556
_database_code_amcsd             0020370
_diffrn_ambient_pressure         9.17e+06
_exptl_crystal_density_diffrn    3.948
_cod_data_source_file            inputs/fixed/downloads/05/05852.cif
_cod_data_source_block           05852
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017131
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p14 Note: P = 9.82 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017132
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p14
 Note: P = 9.82 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7087
_cell_length_b                   4.7087
_cell_length_c                   14.9313
_cell_formula_units_Z            6
_cell_volume                     286.702
_database_code_amcsd             0020371
_diffrn_ambient_pressure         9.82e+06
_exptl_crystal_density_diffrn    3.974
_cod_data_source_file            inputs/fixed/downloads/05/05853.cif
_cod_data_source_block           05853
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017132
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p15 Note: P = 10.88 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017133
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p15
 Note: P = 10.88 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7017
_cell_length_b                   4.7017
_cell_length_c                   14.855
_cell_formula_units_Z            6
_cell_volume                     284.389
_database_code_amcsd             0020372
_diffrn_ambient_pressure         1.088e+07
_exptl_crystal_density_diffrn    4.006
_cod_data_source_file            inputs/fixed/downloads/05/05854.cif
_cod_data_source_block           05854
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017133
The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p16 Note: P = 11.90 GPa
Merlini, M.; Hanfland, M.; Gemmi, M.; American Mineralogist 100 (2015) 2625–2629; doi:

data_9017134
_publ_section_title
;
 The MnCO3-II high-pressure polymorph of rhodocrosite
 Note: Sample run2-p16
 Note: P = 11.90 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              2625
_journal_page_last               2629
_journal_volume                  100
_journal_year                    2015
_chemical_compound_source        'Sardegna, Italy'
_chemical_formula_sum            'C Ca0.04 Mn0.96 O3'
_chemical_name_mineral           Rhodocrosite
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.6955
_cell_length_b                   4.6955
_cell_length_c                   14.7918
_cell_formula_units_Z            6
_cell_volume                     282.433
_database_code_amcsd             0020373
_diffrn_ambient_pressure         1.19e+07
_exptl_crystal_density_diffrn    4.034
_cod_data_source_file            inputs/fixed/downloads/05/05855.cif
_cod_data_source_block           05855
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mn.96 Ca.04) C O3'
_cod_database_code               9017134